Science &amp; Engineering A

## Manuscript Draft

Manuscript Number:

Title: IONIC CONDUCTIVITY OF SOLID OXIDES HxAg1-xTaWO6.nH2O: MICROSTRUCTURAL ASPECTS

Article Type: Research Paper

Keywords: Empirical models; impedance spectroscopy; easy-path model

Corresponding Author: Dr. Daniel Valim, Ph.D.

Corresponding Author's Institution:

First Author: Daniel Valim, Ph.D.

Order of Authors: Daniel Valim, Ph.D.; Antônio G Souza, Ph.D.; Josue M Filho, Ph.D.; Oswaldo L Alves, Ph.D.; Eder N Silva, Ph.D.; Marco Aurelio C de Santis, Ms; Romildo J Ramos, Ph.D.

Abstract: A study of impedance spectroscopy was done for the electrical characterization of pyrochlore materials. The experiment consisted of measurements of the dependence of the impedance of such systems with the temperature during heating (25 to 110 °C) and cooling (110 to 25 °C). The goal was to try to avoid the effect of humidity in the impedance spectrum. However, for the sample with x = 0.20, we get an anomalous response of the conductivity during the cooling process. To explain this result, we performed micro-structure characterization in this sample and in the samples with x = 0.80 and 0.67. The result is that the sample with x = 0.20 is well characterized by the model "easy-path'' because it has high porosity while the other two must have phase precipitate structure type Suzuki. These results served to explain why the anomaly on the Arrhenius plot occurred only in the 0.20 concentration sample: microstructure difference. In this study we can also note that the doped samples had a dependence of activation energies related to the rates of concentration. Except for the sample with concentration rate of 0.20, the activation energies during cooling are among the values of 0.60 and 0.23 eV of their pure counterparts which are registered in the literature.

Research Data Related to this Submission --------------------------------------------------

There are no linked research data sets for this submission. The following reason is given:

The authors do not have permission to share data

## IONIC CONDUCTIVITY OF SOLID OXIDES HxAg1-xTaWO6.nH2O: MICROSTRUCTURAL ASPECTS

D Valim - Depto. de Matemática - UNEMAT/ Sinop, Brazil e-mail: daniel.valim@unemat.br

-  AG Souza Filho - Depto. de Física  - UFC/ Fortaleza, Brazil
-  JM Filho - Depto. de Física  - UFC/ Fortaleza, Brazil
-  OL Alves - Depto. de Química - UNICAMP/Campinas, Brazil
-  MAC de Santis - Depto. de Química - UNICAMP/Campinas, Brazil
-  EN Silva - Depto. de Física - Universidade Federal do Maranhão/ São Luíz, Brazil
-  RJ Ramos - Instituto de Física - Universidade Federal do Mato Grosso/ Cuiabá,  Brazil

Abstract : A  study  of  impedance  spectroscopy  was  done  for  the  electrical  characterization  of pyrochlore  materials. The  experiment  consisted  of measurements  of  the  dependence  of  the impedance of such systems with the temperature during heating (25 to 110 °C) and cooling (110 to 25 °C). The goal was to try to avoid the effect of humidity in the impedance spectrum. However, for the  sample  with  x  =  0.20,  we  get  an  anomalous  response  of  the  conductivity  during  the  cooling process.

To  explain  this  result,  we  performed  micro-structure  characterization  in  this  sample  and  in  the samples with x = 0.80 and 0.67. The result is that the sample with x = 0.20 is well characterized by the model 'easy-path'' because it has high porosity while the other two must have phase precipitate structure  type  Suzuki.  These  results  served  to  explain  why  the  anomaly  on  the  Arrhenius  plot occurred only in the 0.20 concentration sample: microstructure difference. In this study we can also note  that  the  doped  samples  had  a  dependence  of  activation  energies  related  to  the  rates  of concentration. Except for the sample with concentration rate of 0.20, the activation energies during cooling are among the values of 0.60 and 0.23 eV of their pure counterparts which are registered in the literature.

Keywords: Empirical models, impedance spectroscopy, "easy path" model.

## INTRODUCTION

The  group  of  pyrochlore  is  chemically  diverse.  Hogarth  cited  by  Chelgani[1]  defined  the formula of pyrochlore oxides as A2-mB2O6  1-n .pH2O where A represents an element mono-, di-, or trivalent, B represents an element tri-, tetra-, penta-, or hexavalent and  =O, OH, F. The structures of  pyrochlore  may  vary,  depending  of  the  cation  distribution  in  sites  A  and  anions  in  sites  ,  as normal, ideal, defective and reverse. For normal pyrochlore there is a regular distribution of atoms on the A sites (at positions 16d, Wyckoff notation) and  (at positions 18b). A typical pyrochlore has an intermediate structure between the ideal and defective structures, which are set to m = 0 (complete A cation)  and  m  =  2  (absent  A  cation).  Some  of  the  normal  pyrochlore's  related  structures  show  an inverse  distribution  of  A  cations  and  site  vacancies,  namely  the  A  cations  (with  m  &lt;1)  occupy positions 8b while the vacancies occupy the positions 16d.

The compounds under investigation in this work are of type m = 1, n = 1, p = 0, 0.5 or 1. Many pyrochlores  with  the general chemical  formula  AB'B'O6,  as  the  HTaWO6  [2]  has  random distribution of cations B' and B" in the center of the octahedrons. These compounds crystallize in the space  group  Fd3m(Oh 7 )  and  belong  to  a  class  of  materials  with  450  synthetic  compositions  with properties  that  include:  catalysis,  piezoelectricity,  iron  and  iron  magnetism,  luminescence  and colossal magnetoresistance [3,4]. Other pyrochlores exhibit another collection of interesting physical properties such as semiconducting and superconductivity [5,6]. In this structure the atoms B and X form  a  matrix  of  octahedral  (BX6)  connected  by  vertices  while  Y  and  A  form  another  array  of tetrahedral  (YA4) sharing vertices.  This  structure  is  analogous  to  other  types  of  structures  such  as those of the ReO3 and perovskite CaTiO3. However, in the pyrochlore the unit skeleton (BO6)n is more complex and the cavities left by them are more open than in the other two cases. These cavities have an average diameter between 3.8 and 4.6 Å[7].

The  defective  pyrochlores  belong  to  a  class  of  cationic  materials  that  have  been  extensively studied  in  the  last  years,  such  as  in  the  search  for  good  solid  ionic  conductors  for  technological applications [8] as for model systems to study ion conduction[9]. For this reason, the characterization technique used in this paper has been  Impedance Spectroscopy.  Impedance spectroscopy (IS) is a versatile,  non-destructive  and  non-evasive  technique,  able  to  both  electrical  measurements  and microstructural  characterizations.  For  the  ionic  conductions  mechanism  studies,  this  technique  is very  useful  to  understand  it.  Because  the  microstructure  of  the  material  is  easily  described  by electrical models used to fit the electrical curves obtained by IS technique.

The  correct  interpretation  about  IS  variables  depend  on  the  correct  previous  model.  In  a crystalline  idealized  solid,  the  model  for  both  impedance  and  permittivity  is  the  Debye  one  [10]. However, in polycrystalline solids, where there is presence of micro or nano crystals, some effects associated with the material roughness, the grain borders or simply distribution in activation energies in  ionic  monocrystalline  conductors  appear  [11].  In  the  case  of  polycrystalline  materials,  such  as those  studied  in  this  work,  the  CPE  effect  is  associated  to  the  microstructure  (microcrystals  and borders of microcrystals).

In order to characterize materials by impedance spectroscopy, we use equivalent circuit models, where the elements represent physical processes that occur in a material, and which together allows us to understand and classify the physical properties of the studied material. In this work, we have shown the results of ionic conduction studies through impedance spectroscopy characterization of HxAg1-xTaWO6.nH2O pyrochlore samples, take into account both intrinsic and extrinsic mechanisms.

## 1 EXPERIMENTAL PROCEDURE

## 1.1 Sample Synthesis

The  pyrochlore  precursor  KTaWO6  samples  were  synthesized  via  solid-state  reactions  from stoichiometric amounts of the reactants. The reactants were K2CO3(Riedel - 99%), Ta2O5 (Alfa 99%)  and  Tungsten  oxide  WO3  (Aldrich)  with  99  %  of  purity.  The  reagents  and  their  both manufacturer and purity is shown in Table 1 .

The reactions can be viewed as follows:

The procedure is an adaptation of procedure described by Mari[12]. The reagents were crushed and mixing in an agate mortar for 10 minutes. The system remained under heating for 45 hours, and every 15 hours the reaction was stopped for crushing and homogenization of the mixture.

Table 1. Characteristics of used reagents.

| Reagent             | Formula   | Manufacturer   | Purity(%)   |
|---------------------|-----------|----------------|-------------|
| Tantalum Dioxide    | Ta 2 O 5  | Alfa           | 99          |
| Tungsten Oxide      | WO3       | Aldrich        | 99          |
| Potassium Carbonate | K 2 CO 3  | Riedel         | 99          |
| Silver Nitrate      | AgNO 3    | Merck          | 99.8        |
| Nitric Acid         | HNO 3     | Aldrich        | 65*         |
| Hydrochloric Acid   | HCl       | Merk           | 36.5-38*    |

The  pyrochlore  HTaWO6.H2O  compound  was  obtained  by  ionic  exchange  reaction  between KTaWO6 and a 12 mol.L -1 HCl solution. The system was left under stirring at room temperature for 48 hours, with two exchanges of the supernatant solution after centrifugation of the solid.

The HTaWO6 was submitted at new ionic exchange reaction. The proton ion was exchanged by Ag + to make AgTaWO6. The reactions were performed using the procedures of LQES laboratory for similar  compounds  [13,14].  In  this  part  of  work,  the  reactions  were  optimized  for  a  maximum exchange proton-silver. The compounds were dipping in AgNO3 solution with a concentration of 10 -3 at 10 -2 mol.L -1 and stirring by magnets at room temperature during 48 hours.

Finally, the protonated compounds were again subjected to ion exchange reactions, this time the proton  was  replaced  by  Ag   ions.  The  reactions  were  performed  using  the  procedures  of  LQES + laboratory  for  similar  compounds  [13,14].  For  this  time,  the  reactions  were  performed  by  molar rations of 4:1, 2:1, 1:1, 1:2, 1:4 and 1:8 to form H1-xAgxTaWO6.H2O.

The compounds were immersed in aqueous AgNO3 solutions and magnetically stirred at room temperature  for  48  hours.  The  solids  were  then  separated  by  centrifugation  and  washed  with deionized water. The washing and purification process was repeated three times.

Our work consisted of a similar study of reference [15], where the HTaWO6 pyrochlore samples were submitted substitutional homovalent doping with silver by an ion exchange reaction, i.e., the proton of the compound was replaced by Ag  to form compounds of type H1-xAgxTaWO6 [16]. The + reactions were performed using the procedures of LQES laboratory for similar compounds [13,14]. The molar ratio H:Ag of each of the samples were 4:1, 2:1, 1:1, 1:2 and 1:4, the code samples are

HAg1:0.25,  HAg1:0.5  ,  HAg1:1,  HAg1:2  and  HAg1:4.  We  know  the  ion  exchange  reaction,  to 4:1(Hag1:0.25) for example, occurs as follows

Where  we  can  adjust  the  x,  which  is  the  concentration  ratio  of  silver  to  0.2.  For  the  other compounds, with names HAg1:0.5, HAg1:1, HAg1:2 and HAg1:4, x values are 0.33, 0.50, 0.67 and 0.80, respectively.

## 1.2 X-ray diffraction

After  sample  synthesis,  the  X-ray  diffractogram  was  obtained  in  a  Shimadzu  diffractometer, operating  in  scan  mode  with  CuKα  radiation,  generated  at  40  KV  and  30  mA  current  [16].  The scanning speed used was 2/min in 2θ, with accumulation for reading every 0.6 seconds. The slits used were: divergent 1.0 mm and collection 0.3 mm. The calibration of the scanning angle was done with polycrystalline silicon and the samples were analyzed in powder form.

In the Figure 1 is shown the X-ray diffraction pattern for all H1-xAgxTaWO6.nH2O pyrochlore samples.  We  can  see  all  peak  indicate  that  structures  belong  to  the  Fd3m  (Oh 7 )  space  group,  in according with reference [17], with eight molecules per unit cell. No significant structural change occurred beyond variations in relative intensities to specific peaks.

70

Figure  1 : X-ray  diffraction  patterns  for  all  samples  synthesized  in  the  LQES  laboratory.  The asterisks indicate the peaks where there are significant changes in the intensities[16].

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-0cddffaa-a384-428f-82a8-986a5b4f1b06.jpg)

## 1.3 Impedance Spectroscopy

The impedance spectroscopy measurements with temperature dependency were made on four samples  H1-xAgxTaWO6.H2O  pyrochlore.  The  experiments  have  performed  in  the  laboratory  of electrical  measurements  of  the  Physics  Institute  of  the  Federal  University  of  Mato  Grosso.  The experimental method consisted of impedance measuring of samples within a frequency range from 1 Hz  to  1MHz  for  each  temperature,  both  as  heating  and  cooling.  The  range  of  temperatures  was between 25° C (27° C) and 110° C (105 or 120° C) depending upon the sample. The heating and cooling  procedures  have  performed  to  study  the  conductivity  and  the  activation  energies  for  both processes.

The experimental apparatus has consisted of an impedance analyzer Solartron Analytical model 1260, Solartron Analytical 1296 dielectric interface and a commercial oven with sample holders. The diameter of the electrodes was 10 mm for samples HAg1:1 HAg1:0.5, but it was 3 mm in diameter for the other samples due to the small size of them. The thickness of each sample was 0.6 mm for the samples HAg1:0.5; HAg1:1; HAg1:4 and HAg1:0.25 and 0.65 mm for HAg1:2. As a consequence, the relation between thickness and area (electrode area) l/A was 0.076 cm -1 for samples HAg1:1 and HAg1:0.5, 0.92 cm -1 for HAg1:2 and 0.85 cm -1 for samples HAg1:4 and HAg1:0.25. These values are used to determine the real and imaginary conductivities used in log-log curves of conductivity. We have obtained the conductivities  (real  and  imaginary)  from  the  experimental  data  of  real  and imaginary impedance through the following expressions:

$$\sigma ^ { \prime } = \frac { 1 } { A } \frac { Z ^ { \prime } } { \left ( Z ^ { ^ { \prime } 2 } + Z ^ { ^ { \prime } 2 } \right ) }$$

and

$$\sigma ^ { \prime \prime } = \frac { 1 } { A } \frac { Z ^ { \prime \prime } } { \left ( Z ^ { \prime ^ { 2 } } + Z ^ { \prime ^ { 2 } } \right ) }$$

Where  ' is the real conductivity, and  " is the imaginary conductivity. The real conductivity was the greatness used to obtain the activation energies of the pyrochlore samples.

## 2 Results and Discussion

## 2.1 Activation Energies

The parameter  dc is thermally activated, having an Arrhenius type behavior, given by:

$$\begin{smallmatrix} & & \\ & & \\ 8 \end{smallmatrix}$$

Equation 8 describes the conductivity in the region where the defects are formed and moved, and there is a single kind of defect formed. If there is more than one type of charge carrier, this equation must be rewritten for all the different conduction mechanisms, considering its exponents and relevant pre-factors [18].

If we make manipulations in equation 8, multiplying it by T and by taking the decimal logarithm on both sides of the equation, we obtain the following equation:

$$\begin{smallmatrix} & & \\ & & \\ 8 \end{smallmatrix}$$

Where is the Arrhenius equation, valid for all models of ion conduction. The graph of log (  T) versus 10 /T is a straight line whose slope is given by 4  E/(1,985[eV/K]).

Figure 2: Arrehnius plot for ionic conduction for H-1-x AgxTaWO6.H2O samples.  (a) Cooling process. (b) Heating process. Numbers represents activation energies and pre-factor  0 respectively .

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-b81f1145-0d24-49d5-aa90-ef84c42f9432.jpg)

In Figure 2 (a) and (b) it is shown the Arrhenius plots for all samples studied for the processes of heating and cooling, respectively. We have calculated the activation energies by the linear fitting of curves  shown  in  these  figures.  The  results  of  this  linear  fit  for  all  samples  present  the  following characteristics:

-  The activation energy during heating for the samples were 0.30, 0.37, 0.55, 0.47 and 0.28 eV for the samples with x = (0.80, 0.67, 0.50, 0.33 and 0.20) respectively;
-  The activation energies during cooling are 0.35, 0.45, 0.57 and 0.59 for the samples with x = (0.80, 0.67, 0.50 and 0.33), respectively;
-  The negative curve slope (-0.62) for x = 0.20 shows that a thermally activated process did not  occur.  It  is  an  abnormality  that  occurs  in  a  hygroscopic  material  [19,20,21,22] associated with the material hydration [19,21];
-  The increased doping reduces the activation energy during the heating process;
-  During cooling, the samples had greater activation energies than those during heating;
-  The differences in activation energy between the processes of heating and cooling for each sample  are  0.05,  0.08,  0.02  and  0.12  for  samples  with  x  =  (0.80,  0.67,  0.50  and  0.33), respectively. The biggest difference in activation energy is in the sample with x = 0.33;
-  During both heating and cooling the activation energies for these samples are within the range  of  values  reported  in  Reference  [23]  for  the  pure  compound  HTaWO6  between hydrated  and  anhydrous  forms  (0.27  and  0.66  eV).  It  is  a  strong  indication  of  the dependence of activation energy with doping.

By carefully examining the Arrhenius curve of the sample with rate concentration x = 0.20, we note that there is a discontinuity in it between the temperatures of 70-60 ºC, where the points form two lines above and below the temperature of 70 ºC. The region from 70 to 100 °C is where  the water loss process by  grains  boundary  surface dominates as seen in Chapter 1 of Reference [24]. Below this region is the reverse process: water condensation. We have, therefore, a strong evidence water condensation effect in the grain boundary.

## 2.2 Characterization of microstructure

Figure 3: The model used for characterizing x = 0.20 sample, showing both complex impedance plot and equivalent circuit.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-8eae4396-927c-4364-89a6-db91876161e9.jpg)

Figure 4 (1) and (2) shows the effect of grains and grain boundary for the samples with x = 0.80 (heating  and  cooling)  and  0.20  during  cooling,  respectively.  Since  the  time  constants  for  each conduction process (grain and grain boundary) are very close, in sample x = 0.80 it only appears one impedance arc, as for the module, it seems a superposition of two arcs. For the sample with x = 0.20, the situation is the opposite. This situation is analogous to that shown in reference [10], where the author highlights the investigation in both impedance arcs and the electrical module to characterize materials by its microstructure. This effect also appears for the sample with x = 0.67 but not for the samples  with  x  =  0.50  to  0.33  where  there  is  no  resolution  in  grain  boundary  (see  Figure  5).

Figure 4: Impedance (a) and electric Modulus (b) for (1) x = 0.80 and (2) 0.20. Similar case of references [1,16].

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-3f0251ae-b525-4069-b2b5-d3cc97dd6108.jpg)

The electrical modulus response of the sample with x = 0.80 is typical of compounds with the Suzuki type phase, which consists of the solid-state precipitates forming islands on a second stage matrix [25]. As shown in the reference, the overlapping of complex modulus arcs indicates grains larger than 1 µm. As for the sample with x = 0.20, the microstructure is the one with grains very close to each other, i.e., very narrow grain boundary.

To confirm that, we use an equivalent circuit model to characterize the impedance of the sample with  x  =  0.20.  The  model  consists  of  two  parallel  lines,  R-CPE  connected  in  series,  as  shown  in Figure  3.  From  this  model,  we  made  the  adjustments  for  the  complex  impedance  curves  for  the referred sample obtained during cooling between the temperatures of 110 and 25 ºC.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-4839c3fd-f0d6-4a6b-b0d4-82037e072e22.jpg)

Figure 5: Impedance (a) and Electric Modulus (b) for (1) x = 0.50 and 0.33 and (2) x = 0.67.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-38bd5739-0aed-4242-9c9a-1beb573dd977.jpg)

The author of reference [10] in Chapter 4 of his book describes various physical models used for materials characterization. The models described range from the simplest (layers) to more complexes ones (Maxwell-Wagner). To characterize the sample with x = 0.20, we use two intermediate models: 'brick-layer''  and  'easy-paths.'  The  first  consists  of  a  tri-dimensional  matrix  of  cubic  grains separated by grain boundary of plane layers with a certain thickness [10], while the second consists of irregularly shaped grains where there is a region of electrical contact between them (see Figure 6).

In  the  'brick-layer'  model,  we  generally  assume  that  there  is  a  region  of  continuous  phase separated by individual grains. However, often where the conductivity of the grain interior is larger than  the  grain  boundary    (  ig &gt;  cg )  it  is  observed  that  the  activation  energies  are  equal  or  very similar  [10].  This  observation  led  Bauerle  [26]  to  suggest  that  there  are  regions  where  the  grain contours form good intergranular electrical contacts; it is called easy paths (see Figure 6).

Figure 6: Two easy models for ceramics: (a) Schematic models representation for grain versus discontinuous grain boundaries. (b) Equivalent series circuit according Baurle(1969). (c) Parallel circuit according Schouler (1970)[10,27].

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-01fa0705-d7d7-4489-8d48-8a2313822aaa.jpg)

Bauerle's  idea  is  that  the  migrant  oxygen  ions  are  sequentially  and  partially  blocked  in  the grain's  interiors  and  boundary.  Thus  there  only  remains  the  restriction  of  easy  ionic  paths  (easy- paths). Since the contour permittivities and grains' interiors are equal or approximately equal (  ig =  cg ) , the existence of little intergranular contact could not noticeably affect the capacitance Ccg [10].

A slightly different model was proposed by Schouler [27]. As shown in Figure 6(c), the model divides the ionic current into two paths, one of which the conductance and capacitance (Gcg e Cig, respectively), are capacitively blocked, while another (Ga) is not. The ratio of blocked ionic current is given by

$$\begin{smallmatrix} & & \\ & & \\ 9 & & \\ \end{smallmatrix}$$

Circuitry (b) and (c) of Figure 6 are equal, as shown in Chapter 1 of reference [10]. Thus, the rate  can be expressed using the equivalent circuit series

$$\begin{smallmatrix} & & \\ 1 0 \end{smallmatrix}$$

When we have a situation where the activation energies for grain and grain boundary are equal (see section 3.1), the parameter  also  serves  to  estimate  the  percentage  with  which  the  grain  is covered by grain boundary phase, i.e., the percentage of the grain surface area that is covered by the second phase. In the case of the sample with x = 0.20 at the temperature of 100 ° C during cooling the parameter  is:

$$\beta = 0, 8 3,$$

i.e., for the sample with x = 0.20, 83% of the grain surface is covered by a second grain boundary phase. This means that electrical contact between grains is only 17% of the total surface area. But this  is  only  an  estimate.  The  results  presented  here  need  to  be  confirmed  through  studies  of  the technique of Scanning Electron Microscopy.

The  microstructural  arrangement  above,  allows  that  a  small  amount  of  condensed  water  can causes a large change in the ionic conductivity of the material.

But to understand how water condensation on surfaces of grain boundary produces observable effect, it is necessary to take into account our knowledge of microstructure. The sample with x = 0.20 can have grain boundary microstructure with enough reduced volume so they can have contact points with each other ('' easy path').

Figure 7 shows the Arrhenius plot of the grain resistance (Rig) and grain boundary (Rcg) for the sample  with  x  =  0.20,  and  whose  values  and  range  of  temperature  are  shown  in  Table  2.  The Arrhenius plots shown in the before said Figure are similar to those shown in the references [10] and [19].

Figure 7: Arrhenius plot for inter and grain-boundaries resistances (x=0.20 sample). The graphic shows two regions: easy path and grain boundaries.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-6bb8b4e6-c4df-4d79-b84a-5c45c54e8211.jpg)

In the region of the conductivity of the grain boundary, the resistance grain boundary resistance Rcg is much larger than the grain interior one Rig and the angular coefficients of the straight lines are 0.32 and 0.23, therefore, very close. In the conduction region 'easy path,' coefficients are 0.015 and  0.008  for  the  resistance  of  interior  and  grain  boundary,  respectively.  The  error  for  each coefficient is 0.02; namely, the 'activation energies'' are about equal. In the previous section, we saw that Bauerle [26] used this property to explain the conduction model of 'easy paths.' The fact that there  are  points  where  grains  have  electrical  contact  illustrates  the  fact  that  there  are  activation energies of grain and grain boundary equal or similar to each other [10].

In the conduction region 'easy path' the dominant thermal process is water evaporation. But as we lower the temperature, we get more water condensation, which increases the electrical contact between the grains, reducing the resistance, in an inverse process to the increasing resistance of the grains. The result is practically constant electrical resistance in this range of temperature. However, in  the  conduction  region  of  the  grain  boundary,  there  is  a  process  wherein  the  grain  boundary dominates ionic conduction of the material. In this region, as well as the other one, it does not make sense  to  talk  about  activation  energies,  once  it  coincides  with  the  ones  that  dominate  water condensation. It means that the more we lower the temperature, the more surface water will be in the material,  increasing  conductance.  Therefore,  the  'activation  energy''  for  the  sample  with  x  =  0.20 appears negative, when in reality it is not occurring a thermally activated ionic conduction process in it.  What  occurs  is  that  water  condensation  on  the  grains'  surface  eventually  produces  conductive paths percolation in a much faster process than the one with a decrease in conductivity of the grains.

In Figure 8, we can see the activation energy reduction with the increase of doping during the cooling process.

Figure 8: Activation energy and Log  0 versus x plot for both (a) heating and (b) cooling route.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00594v1-figure-1e03635c-1e0d-4194-872a-800490f0a2f2.jpg)

These  results  indicate  that  the  material  HTaWO6.nH2O  doped  with  silver,  whose  formula becomes  H1-xAgxTaWO6.nH2O,  has  as  an  ion  conductor  the  H   and  not  the  Ag .  The  results + + discussed in Chapter 3 of Reference [24] indicate that the Ag  cannot be the carrier; otherwise, the + material  would  degrade  in  the  TaWO5.5  compound.  Besides,  among  the  various  conduction mechanisms cited in Reference [24]: jumps, tunneling, mixed (jumps and tunneling) [23], Grothus effect [29] and the effect of surface water in the grain boundaries [29], only jump conduction and conductivity by surface water of grain boundary are possible in our samples.

The introduction of ion Ag  on 16c site weakens the bonds of octahedral Ta-O and W-O that + surround the structure, reducing the vibration frequencies of the octahedral [24], which as a result, cause an enlargement of the potential wells existents within the channels where the hydrogen atoms are localized. This describing take into account the hard-core atomic model. Although it seems very unrealistic, we note in Reference [23] that an ion exchange from site 16c to another one with larger ionic ratio increases the unit cell volume and thus facilitate the conductivity. The authors showed that for  a  homovalent  cation  replacement  Gd 3+ for  Er 3+ ,  Y 3+ ,  Dy 3+ ,  Sm 3+ ,  and  La 3+ ,  ion  conductivity decreases monotonically  as the average  size of the cation increases[23]. The  authors also demonstrate that the material having less distension ('stress') produced by the doping atom is the one that has the highest conductivity. In our case, we found that the sample with x = 0.80, one of the samples with the lowest disorder, is the sample that has higher activation energy.

The decrease in activation energy with the doping increase is related to a compromise between two opposing processes. The first is the  enlargement of the channels formed by octahedral in the directions [110] caused by the presence of Ag  ions, and the second is the blockage exercised by + them.  The  silver  ions  do  not  take  part  in  the  conduction,  as  it  has  been  seen,  blocking  proton conduction. Thus, the probability of an H  ion to find an Ag  ion blocking its path, restricting the + + possible ways that can be traversed in the structure increases with the concentration rate of Ag . +

In a pure material (HTaWO6), the most probable paths for conducting protons are all those that pass through the parallel channels the directions [110], which for a face-centered cubic structure are all those six directions that pass through the diagonal edges of a cube. In the case of the sample with silver rate concentration equal to 0.80, the probability of an ion H + in the center of the cube to find as a  first  neighbor  a  second  ion  H + or  the  vacancy  of  it  (which  would  allow  conduction)  is  0.2x0.2, which is 0.04, i.e., 4%. This last one, on the other hand, has an equal probability of finding another H + ion, and this ion has 0.04 probability of finding another one, and so on, making a random path between the Ag  ion similar to a labyrinth. +

The  problem  that  relates  possible  random  ways  on  two  or  three-dimensional  networks  is  the percolation,  which  has  established  a  minimum  lower  limit  on  the  probability  of  a  physical  being finding a full path in a finite network, which depends on the freedom degrees and the used geometry. In the case of a face-centered cubic structure, such as the pyrochlore ones, the minimum percolation limit is 0.2 [30], meaning that the probability of an H + ion to find another in 0.2 is the minimum limit so  percolation  can  happen.  So,  for  silver  concentration  rate  of  0.80,  we  are  almost  at  the  limit  of optimization of the ionic conductivity. It means that for the Ag  ion as doping, we can increase the + concentration rate to 0.90.

## 3 CONCLUSION

The activation energies during cooling are within lower and upper bounds for pure samples, in their anhydrous (0.60 eV) and hydrated (0.23 eV) forms. This result indicates that doping with silver influence in decreasing the activation energy.

The  doping  of  the  compound  HTaWO6  with  Ag   increases  the  ionic  conductivity.  The + explanation is that the presence of Ag  Ion extends the channels around the H  ions, facilitating the + + conduction [23]. The sample with x = 0.20 showed anomalies during cooling. The results plotted in the low-temperature region are similar to that reported in the literature by several authors [19-22]. The microstructure characterization indicates a possible structure 'easy-paths' type, which needs to be confirmed by further studies of Scanning Electron Microscopy. For this sample, it is also required a study in Impedance Spectroscopy with a controlled atmosphere temperature.

## 4 ACKNOWLEDGMENTS

D.V.  and  A.G.S.F.  acknowledge  financial  support  from  the  Brazilian  agencies  CNPq  and FUNCAP. We would like to thank Dr. R. J. Ramos (UFMT) for laboratory facilities, for Impedance Spectroscopy measurements.

## REFERENCES

- [1] S. C. Chelgani et. al, Minerals Engineering 55 , 165-171 (2014).
- [2] D. GROULT, B. RAVEAU, and C. MICHEL, COMPTES RENDUS HEBDOMADAIRES DES SEANCES DE L ACADEMIE DES SCIENCES SERIE C 274 , 374.
- [3] M.A. Subramanian, G. Aravamudan, and G.V.S. Rao, Prog. Solid State Chem. 15 55-143 (1983).
- [4] M.A. Subramanian, B.H. Toby, A.P. Ramirez, W.J. Marshall, A.W. Sleight, and G.H. Kwei, Science 273 (1996) 81-84.
- [5] B.J. Kennedy, T. Vogt, J. Solid State Chem. 126 (1996) 261-270.
- [6] S. Yonezawa, Y. Muraoka, Y. Matsushita, Z. Hiroi, J. Phys.: Condens. Matter 16 (2004) L9L12.
- [7] C.  M.  Mari,  F.  Bonino,  M.  Catti,  R.  Pasinetti,  and  S.  Pizzini,  Sol.  Stat.  Ion. 18-19 ,  1013 (1986).
- [8] J.  Hidalgo, M. Colet-Lagrille, and A. Mukasyan, Cryst. Res. Technol. 50 ,  No. 11, 879-883 (2015).
- [9] M. Catti, C. Mari, and G. Valerio, Journ. Sol. Stat. Chem. 98 , 269 (1992).
- [10]J. R. Macdonald, Impedance Spectroscopy Emphasizing Solid Materials and Sistems , JOHN WILEY SONS, 1 edition, 1987.
- [11]C. Leon, M. L. Lucia, and J. Santamaria, Physical Review B 55 , 882 (1997).
- [12]C. M. Mari, M. Catti, and M. Castelli, A Characterization of KTaWO6.H2O. Mat. Res. Bull., v.21. p. 773-778, (1986).
- [13]Zarbin, Aldo J G, Alves, Oswaldo L, Amarilla, J Manuel, Rojas, R M, and Rojo, J.M, Chem. Matter. V. 11, p. 1652-1658, (1999).
- [14]A. Galembeck, and O.L. Alves. J. Mater. Sci, v.34, p. 3275-3280, (1999).
- [15]J A Díaz-Guillén, A F Fuentes, M R Díaz-Guillén, J M Almanza, J Santamaría, and C Léon, Journal of Power Sources 186 , 349 (2009).
- [16]M. A. C. de Santis, Estrutura lamelar versus estrutura pirocloro: Obtenção de compostos do tipo H1-xAgxTaWO6, Master thesis, UNICAMP-Universidade Estadual de Campinas, 2006.
- [17]C. M. Mari, M. Catti, and M. Castelli, A Characterization of KTaWO6.H2O. Mat. Res. Bull., v.21. p. 773-778, (1986).
- [18]E. N. Silva, Espectroscopia vibracional e de impedância em monocristais de SrAlF5, Master thesis, Universidade Federal do Ceará, 2005.
- [19]C.  M.  Mari,  F.  Bonino,  M.  Catti,  R.  Pasinetti,  and  S.  Pizzini,  Sol.  Stat.  Ion. 18-19 ,  1013 (1986).
- [20]C. M. Mari, M. Catti, A. Castelli, and F. Bonino, Mat. Res. Bull. 21 , 773 (1986).
- [21]M. Catti, E. Cazzanelli, C. M. Mari, and G. Mariotto, J. Solid State Chem. 107 , 108 (1993).
- [22] M. Catti and C. M. Mari, Sol. Stat. Ion. 40/41 , 900 (1990).
- [23] M.A. Butler and R. M. Biefeld, Phys. Rev. B 19 , 5455 (1979).
- [24] D.  Valim, Espectroscopia  vibracional  e  de  impedância  de  A1-xA`xTaWO6.nH2O  (A=H,  Li, A'=Ag, H) , PhD thesis, Universidade Federal do Ceará, Fortaleza-CE, 2009.
- [25] N. Bonanos and E. Lilley, J. Chem. Solids 42 , 943 (1981).
- [26] J. E. Bauerle, Journal of Physical Chemistry Solids 30 , 2657 (1969).
- [27] E.  J.  L.  Schouler, Etude  des  Cellules  a  Oxyde  Electrolyte  Solide  per  la  Methode  des Impedances Complexes , Ph.d thesis, Institut National Potytechinique de Grenoble, 2005.
- [28] E. Lilley and J. E. Strutt, Physics State Solid 54 , 639 (1979).
- [29] M. Catti, C. Mari, and G. Valerio, Journ. Sol. Stat. Chem. 98 , 269 (1992).
- [30] C. D. Lorentz and R. M. Ziff, Journal of Physics A 31 , 8147 (1998).
Daniel Valim Antônio G Souza Filho Josue M Filho Oswaldo L Alves Eder N Silva Marco Aurélio C de Santis Romildo J Ramos
Ionic Conductivity Of Solid Oxides Hxag1-xtawo6.NH2O: Microstructural Aspects
A study of impedance spectroscopy was done for the electrical
characterization of pyrochlore materials. The experiment consisted of
measurements of the dependence of the impedance of such systems with the
temperature during heating (25 to 110 {\deg}C) and cooling (110 to 25 {\deg}C).
The goal was to try to avoid the effect of humidity in the impedance spectrum.
However, for the sample with x = 0.20, we get an anomalous response of the
conductivity during the cooling process. To explain this result, we performed
micro-structure characterization in this sample and in the samples with x =
0.80 and 0.67. The result is that the sample with x = 0.20 is well
characterized by the model "easy-path" because it has high porosity while the
other two must have phase precipitate structure type Suzuki. These results
served to explain why the anomaly on the Arrhenius plot occurred only in the
0.20 concentration sample: microstructure difference. In this study we can also
note that the doped samples had a dependence of activation energies related to
the rates of concentration. Except for the sample with concentration rate of
0.20, the activation energies during cooling are among the values of 0.60 and
0.23 eV of their pure counterparts which are registered in the literature.